K. U. Madhu and C. K. Mahadevan / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 4, Jul-Aug 2013, pp.2264-2267
Dielectric Studies Of Manganese Carbonate Nanocrystals K. U. Madhu and C. K. Mahadevan Physics Research Centre, S.T.Hindu College, Nagercoil-629 002, India
Abstract Over the past few years, the synthesis and characterization of nanocrystals of materials have become an area of intense research activity. MnCO3 (Manganese Carbonate) is a well known semi conducting material and is highly useful in electronic and optical devices. In the present study, we have made an attempt to prepare MnCO3 (with two different ratios of preparation) with simple domestic microwave assisted solvothermal method. The samples were characterized by TGA analysis. The particle size determination was done using the XRD pattern. The dielectric studies were carried out. The present study indicates that the polarization mechanism in the nano crystals considered is mainly contributed by the space charge polarization. It can be understood that the space charge contribution plays in important role in the charge transport process and polarizability in all the systems considered in the present study.
Keywords: Manganese corbonate, solvothermal method, dielectric measurements
Over the last few years, the synthesis and characterization of nanocrystals of materials have become an area of intense research activity [1, 2]. Several methods have been reported for the preparation of nanocrystal. MnCO3 (Manganese Carbonate) is a well known semi conducting material and is highly useful in electronic and optical devices. The manganese corbonate nanoparticles can be used as a template for efficient formation of uniform, smooth multilayer polyelectrolyte microcapsules, which are promising systems for biomedical and other applications such as biosensors, bioreactors and drug – delivery devices. The MnCO3 nanocrystals have been prepared by several methods and have been characterized before.Li-Xia Yang have synthesized highly oriented MnCO3 nanocrystal assemblies with an ellipsoidal morphology by ultrasonic solution approach. He Hu et al have synthesized MnCO3 with hierarchical superstructures such as chrysanthemum, straw-bundle, dumbbell and sphere like in water/ethanol system under environment friendly hydrothermal condition. A facile complex homogeneous precipitation method was successfully employed by Shuijin Lei et al for the preparation of MnCO3 and Mn(OH)2 crystals using hydrazine hydrate as the complexing agent in a hydrothermal system. In the present study, we
have made an attempt to prepare MnCO3 with two different ratios of precursors by the simple microwave assisted solvothermal method using a somestic microwave oven . The grain sizes of the samples were determined by using the X-ray powder diffraction data. The AC electrical measurements were carried out.
The analytical reagent grade manganese chloride and urea with ethylene glycol as solvent were taken as precursors for the preparation of manganese carbonate nanopowders. The required amount of substance (A) was estimated by using the formula, A =
MXV (in gram units) 1000
Where M is the molecular weight of the substance, X is the concentration in molar units and V is the required volume of solution. MnCO3 nanopowders were prepared for two molecular ratios of the reactants (precursors). One was mixing manganese chloride and urea in the ratio 1:1 labeled as MnCO3 (1:1) and the next one was mixing manganese chloride and urea in the ratio 1:3 labeled as MnCO3 (1:3). The substances were mixed and dissolved in 200 ml solvent (ethylene glycol) taken in a bowl and kept in a domestic microwave oven. The solution was treated in the microwave oven for about 40 minutes and a colloidal precipitate was formed. The product was cooled naturally at room temperature, then washed with distilled water several times and dried in atmospheric air. The brown precipitate thus formed was again washed with acetone to remove any further impurities present. Thus the pure MnCO3 nanopowders were prepared. The colour of the nanopowders produced was noted. The yield percentage for all the samples were calculated by the formula, Yield percentage =
Total product mass 10 0 . Total reactants mass Using an automated X-ray powder diffractometer (PANalytical) with monochromated CuKα radiation (λ = 1.54056Å) the powder X-Ray diffraction (PXRD) data were collected for the 2 samples. Using the Scherer formula  the grain sizes were determined. The prepared nanocrystals were palletized using a hydraulic press (with a pressure of about 5 tons) and used for the AC
2264 | P a g e
K. U. Madhu and C. K. Mahadevan / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 4, Jul-Aug 2013, pp.2264-2267 electrical measurements. The flat surfaces of the The AC electrical conductivity (ac) was calculated cylindrical pellets were coated with good quality using the relation, graphite to obtain a good conductive surface layer. ac = ε 0 εr ω tan . Using a traveling microscope the dimensions of the Here, ε 0 is the permittivity of free space (8.85 1012 2 -1 pellets were measured. C N m-2) and ω is the angular frequency (ω= 2πf, The capacitance (Cc ) and the dielectric loss where f is the frequency). factor (tan δ) were measured using the conventional parallel plate capacitor method using an LCR meter III. Results and discussion (Agilent 4284A) for the 2 samples with a fixed Figure 1 shows the photograph of the frequency of 1 kHz at various temperatures ranging samples prepared and Figure 2 shows the from 40 - 150°C. The observations were made while corresponding pellets .The preparation time, colour cooling the sample. The temperature was controlled and the yield percentage are given in Table 1. The to an accuracy of ± 1°C. Air capacitance (Ca) was colour of MnCO3 (1:1) nanocrystals observed is dark also measured for the thickness equal to that of the brown and that MnCO3 (1:3) is light brown. The pellet. The area of the pellet in contact with the yield percentage is also significantly high. The electrode is same as that of the electrode. The air results obtained indicate that the solvothermal capacitance was measured only at room temperature method is a considerable one for the preparation of because the variation of air capacitance with MnCO3 nanocrystals. temperature was found to be negligible. The dielectric constant of the pellet sample was calculated using the relation, εr = Cc / Ca. Table 1: Colour, yield percentage, preparation time and observed average grain size Sample MnCO3 (1:1) MnCO3 (1:3)
Colour Dark brown Light brown
Yield percentage [%)] 4.348 10.219
Time taken for preparation [min] 45 40
Observed average grain size [nm] 29 20
Fig. 1 :Powder samples produced: From the left MnCO3 (1:1) and MnCO3 (1:3)
Fig.2 :Pellets of the samples: From the left MnCO3 (1:1) and MnCO3 (1:3)
The PXRD patterns obtained in the present study are shown in Figure 3. The patterns indicate
that the samples prepared are of nanostructured. The average grain sizes are also provided in Table 1.
Fig.3: XRD pattern for MnCO3 (1:1) and MnCO3 (1:3)
2265 | P a g e
K. U. Madhu and C. K. Mahadevan / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 4, Jul-Aug 2013, pp.2264-2267 The dielectric parameters viz. εr, tan δ and ac observed are shown in Figures 4-6. All the parameters increase with increase in temperature.The results obtained in the present study indicate that MnCO3 (1:3) has greater dieleelctric constant than MnCO3 (1:1). The εr observed in the present study (at 40oC with a frequency 1kHz) is about 1.05 for MnCO3 (1:1) and 2.4 for MnCO3 (1:3) which is very small when compared to that of the bulk crystal. The dielectric constant is attributed to four types of polarization which are space charge, dipolar, ionic and electronic . At lower frequencies at which all four types of polarizations contribute, the rapid increase in dielectric constant is mainly due to space charge and dielectric polarizations, which are strongly temperature dependent[8,9]. In the case of 4.0 space charge polarization which is due to the
accumulation of charges at the grain boundary, an increase in polarization results as more and more charges accumulate at the grain boundary with the increase in temperature. Beyond a certain temperature, the charges acquire adequate thermal energy to overcome the resistive barrier at the grain boundary and conduction takes place resulting in decreasing of polarization. This interfacial polarization occurs up to frequencies of around 1 kHz with possibly some contribution from the dipolar polarization also as the temperature increases. The grain size observed for the two systems considered in the present study are less than 30 nm. So it can be understood that the polarization mechanism is mainly contributed by the space charge polarization. 4.0
Temperature ( C)
Temperature ( C)
Fig.4: The dielectric constants
Fig.5: The dielectric loss factors
Temperature ( C)
Fig 6; The AC electrical conductivities Nanoparticles lie between the infinite solid state and molecules. The electrical resistivity of nanocrystalline material is higher than that of both conventional coarse grained polycrystalline materials alloys. The magnitude of electrical resistivity and hence the conductivity in composites can be changed by altering the size of the electrically conducting component. The ac values observed in the present study are very small. When the grain size is smaller than the electron mean free path, grain boundary scattering dominates and hence electrical resistivity is increased. Thus the space charge contribution plays
an important role in the charge transport process and polarizability in the case of all the systems considered in the present study.
MnCO3 (1:1) and MnCO3 (1:3) were prepared by the simple solvothermal method using a domestic microwave oven and characterized by PXRD and dielectric measurements. The yield percentage and the grain size observed indicate that the method adopted for synthesis of the material is best suited for the preparation of MnCO3
2266 | P a g e
K. U. Madhu and C. K. Mahadevan / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 4, Jul-Aug 2013, pp.2264-2267 nanocrystals. The dielectric parameters increase with increase in temperature. The results obtained indicate that the space charge contribution plays an important role in the charge transport process and polarizability.
References  
C.D. Keating, M.J. Natan, Adv. Mater. 45 (2003) 451. L.J. Chen, S.M. Zhang, Z.S. Wu, Z.J. Zhang and H.X. Dang, Mater. Lett. 59 (2005) 3119. Li-Xia Yang, Ying-Jie Zhu, Hua Tong and Wei-Wei Wang. Ultrasonics Sonochem. 2(2007)14 He Hu, Jie-yan Xu, Hong Yang, Jie Liang, Shiping Yang, Huixia Wu, Mat.Res.Bull., 11(2001)46 Shuijin Lei, Zhihong Liang, Lang Zhou and Kaibin Tang, Mater.Chem. Phys. 1(2009)113 K.U. Madhu, T.H. Freeda and C.K. Mahadevan (2009), Intl.J. Mater.Sci. 4(5), 549. B.D.Cullity (1978) Elements of X-ray diffraction (2nd edn.) [Addison Wesley, New York] L.C. Hench and J.K. West (1990) Principles of Electronic Ceramics [John Wiley and sons , NewYork] A.Verma, O.P.Takur, C.Prakash, T.C. Goel and R.G. Mendrinatta, Mater.Sci. Engg. B116 (2005)1.
2267 | P a g e